# First Principles Study of SnO Under High Pressurehigh-pressure research with available experimental...

date post

06-Jul-2020Category

## Documents

view

2download

0

Embed Size (px)

### Transcript of First Principles Study of SnO Under High Pressurehigh-pressure research with available experimental...

First Principles Study of SnO Under High Pressure

M. A. ALI†,ϒ,*, A. K. M. A. ISLAM ϒ,‡, N. JAHAN†, S. KARIMUNNESA† †Department of Physics, Chittagong University of Engineering and Technology, Chittagong-4349, Bangladesh.

ϒDepartment of Physics, University of Rajshahi, Rajshahi-6205, Bangladesh.

‡International Islamic University Chittagong, 154/A College Road, Chittagong, Bangladesh.

This article reports the first-principles study of SnO under high pressure within the generalized gradient approximation (GGA).

We have calculated the structural, elastic, electronic and optical properties of SnO. The elastic properties such as the elastic

constants Cij, bulk modulus, shear modulus, Young modulus, anisotropic factor, Pugh ratio, Poisson’s ratio are calculated and

analyzed. Mechanical stability of SnO at all pressure is confirmed using Born stability conditions in terms of Cij. It is also found

that SnO exhibits very high anisotropy. The energy band structure and density of states are also calculated and analyzed. The

results show the semiconducting and metallic properties at 0 (zero) and high pressure, respectively. Furthermore, the optical

properties are also calculated. All the results are compared with those of the SnO where available but most of the results at high

pressure are not compared due to unavailability of the results.

Keywords: SnO, High pressure, Mechanical properties, Electronic band-structure, Optical properties.

PACS numbers: 71.20.Nr, 71.15.Mb, 60.20.de, 71.20.-b, 78.20.Ci

1. Introduction

In recent times, research based on high-pressure has undergone a new start, permits substantial developments of

high-pressure research with available experimental facility by means of advances in techniques and

instrumentation.1 High-pressure research has drawn huge concentration from researchers due to their vital use to

discover the new types of physical behavior and new potential candidate materials for technological application.

It has also impact on the exploring of previously unexplored chemical and physical properties. Researchers from

many fields of natural sciences like Physics, molecular Chemistry, Geophysics, and Biology, have found an

enormous impact on their respective fields.2-4

To explore and develop the properties of materials under high

pressure it is necessary to identify the different strategies.

SnO is found to be crystallized with tetragonal litharge structure (P4/nmm, S.G. 129, Z = 2). The oxygen

atoms and Sn atoms placed at the Wyckoff position of 2a and 2c site, respectively.5 The tin oxides (SnO and

SnO2) are suitable candidate materials for thin-films processing and applications. Films of these oxides have

become leading important due to their potential applications in solar cells,6 heat reflectors for advanced glazing

in solar applications7,8

and as various gas sensors.9–12

Due to the variety of applications mentioned above, many researchers have paid attentions which are

reported in recent years.13–24

Specially, SnO2, have been largely studied because of its n-type semiconducting

nature with wide band gap (3.6 eV), while research work on SnO are seldom reported due to its decomposing

tendency at high temperature.25,26

But during the last few years researchers have paid their attention. Some

results of experimental and theoretical studies on SnO have been reported. High pressure study of electronic and

structural properties of SnO up to 10 GPa has been studied by Christensen et al.20

Giefers et al21

has investigated

the structural properties of SnO at high pressure up to 51 GPa. The pressure-induced phase transition in SnO has

been studied by Lie et al.22

L. A. Errico23

has studied the structural and electronic properties of SnO and SnO2.

The SnO2 and SnO were investigated by Q J Liu et al.24

First principles studies of SnO at different structures

have also been investigated by Erdem et al.25

It is reported, at zero pressure SnO is a semiconductor but transforms to a metal at 5 GPa.26

Christensen et

al20

reported that a change in the slope of c/a curve as a function pressure was found around 5 GPa which is

responsible for that transition. Recently, a superconducting state of SnO at a pressure, p > 6 GPa is reported27

where a maximum Tc was found 1.4 K at 9.3 GPa. Though a phase transition of α-SnO to γ–SnO under pressure

is reported28–30

but such type of transition is not observed by the recent experiments carried out by Wang et al26

and Giefers et al.21

It was concluded about the phase transition that this might be induced by non- hydrostatic

†M. A. ALI. Department of Physics, Chittagong University of Engineering and Technology, Chittagong-4349, Bangladesh. ‡A. K. M. Azharul Islam. International Islamic University Chittagong, 154/A College Road, Chittagong, Bangladesh. *Corresponding author: M. A. ALI, E-mail: [email protected]

conditions. This motivates us to perform a complete study of SnO under hydrostatic pressure. However, as per

of our knowledge complete study of SnO under high pressure have not been done yet.

Therefore, in this article, a systematic investigation of structural, elastic, electronic and optical properties of

SnO under high pressure is presented. We expect that our study would add novel information on the existing

properties.

2. Computational Methods

The CAmbridge Serial Total Energy Package (CASTEP) code31

is used to perform the calculation of properties

of SnO. The method used in this code is the plane wave pseudopotential approach based on the density

functional theory (DFT).32

During the calculations the exchange-correlation potential are treated within the

GGA using Perdew-Burke-Ernzerhof (PBE).33

A 6 × 6 × 5 k-point mesh of Monkhorst-Pack scheme34

was used

for integration over the first Brillouin zone. The convergence of the plane wave is done with a kinetic energy

cutoff of 500 eV. Excellent convergence is guaranteed by testing the Brillouin zone sampling and the kinetic

energy cutoff which make the tolerance for self-consistent field, energy, maximum force, maximum

displacement, and maximum stress to be 5.0×10-7

eV/atom, 5.0×10-6

eV/atom, 0.01 eV/Å, 5.0×10-4

Å, and 0.02

GPa, respectively. The optimized structure of SnO was obtained using the Broydon-Fletcher-Goldfarb-Shanno

(BFGS) minimization technique.35

3. Results and discussion

3.1. Structural properties and their pressure dependence

Figure 1 shows the crystal structure of tin monoxide (SnO), the tetragonal litherge-type structure (SG P4/nmm,

SG No. 129); in which the position of oxygen atoms are (0,0,0) and (0,0.5,0) of Wyckoff 2a site while the

position of Sn atoms are (0.5,0,u) and (0,0.5,1−u) of 2c site; where the internal parameter u = 0.2361, is a

measure of the position of the O atom along the c-axis. The total energy is minimized by the geometry

optimization of the SnO at zero pressure using CASTEP code. After geometry optimization, the lattice

parameters of SnO are taken at different pressures. The optimized lattice parameters are given in Table 1. Our

calculated results of SnO are compared with the available results.21,24

The calculated lattice parameters are in

reasonable agreement with the experimental results. Considering the nature of GGA-PBE functional, it is not

surprising that theoretical estimates of the lattice parameters and cell volume are slightly higher than the

experimental ones (Table 1).

\Table 1. Lattice constants, a, c, c/a and volume, V of SnO.

Compound Crystal system a c c/a V

SnO Tetragonal

3.90

3.80 3.84

4.95

4.83 4.91

1.27

1.27 1.27

75.95

69.97 72.72

This Cal.

Expt.21 Theo.24

Figure 2 shows the normalized values a/a0, c/c0, c/a and V/V0 of SnO (where a0, c0 and V0 are the structural

parameters at zero pressure) for different pressure. It is seen that the volume decreases with increasing pressure.

Since the tin monoxide is soft materials, therefore it is expected to shrink the volume of the cell when it is pressurized

uniformly. Moreover, the normalized lattice constant c/c0 decreasing more quickly than a/a0 with increasing

Fig. 1. The SnO litharge-type tetragonal structure.

pressures indicating the larger compression along c-axis. A change in the slope of c/a ratio is found around 5

GPa [Fig. 2 (b)], which is reported as an indication of semiconductor to metal transition.20

Our calculated results

are matched well with the results obtained by Giefers et al.21

The interlayer compressibility, d(ln c)/dP =

0.01773312 GPa-1

is about 4.92 times higher than the basal plane linear compressibility d(ln a)/dP = 0.00362235

GPa-1

, also indicates the larger response to the pressure of the lattice constant c than a.

3.2. Elastic properties and their pressure dependence

The independent elastic constants, Cij of SnO are calculated in the pressure range 0 to 25 GPa and are given in

Table 2 along with other results for comparison.25

As per of our knowledge, the elastic constants with limited

pressure (0 to 1.5 GPa) have been reported22

, but for such long pressure range (0 to 25 GPa) is not calculated

before this study. Therefore the comparisons of results obtained at high pressure are not possible at this time.

The finite strain technique has been used to study the elastic properties of SnO. In this case a homogeneous deformation (strain) is applied and resulting stress is calculated. A compound is considered to be mechanically

stable if the values of Cij are all positive and also satisfy the conditions for mechanical stability of tetragonal

crystals:36

C11> 0, C33> 0, C44> 0, C66 > 0, (C11– C12) > 0, (C11+ C33- 2C13) > 0 and [2(C11+ C12) + C33+ 4C13] > 0.

It is found that (Table 2) these conditions are satisfied by SnO and hence mechanically stable.

Table 2. The elastic constants Cij (GPa), bulk modulus, B (GPa), shear modulus, G (GPa), Young’s modulus, Y (GPa), Poisson ratio, ν, and

G/B of SnO under different pressure.

P (GPa)

C11 (GPa)

C12 (GPa)

C13 (GPa)

C33 (GPa)

C44 (GPa)

C66 (GPa)

B (GPa)

G (GPa)

Y (GPa)

ν G/B Ref.

0

92 83 24 35 21 72 43 20 52 0.29 0.46 [This]

147.8 83.9 53.4 102.2 43.9 74.6 86.8 [25]

50 38

20 80 31 [22]

50 [28]

5 131 104 39 76 41 87 71 37 94 0.27 0.52

10 154 126 58 115 57 96 96 45 116 0.29 0.46

15 186 155 91 147 73 105 128 51 135 0.32 0.39

20 204 173 107 167 80 112 145 54 144 0.33 0.37

25 231 188 119 178 96 119 160 63 167 0.32 0.39

The bulk modulus B, shear modulus G, Young’s modulus Y, the Poisson ratio v and Pugh ratio are also

calculated and given in Table 2. Y and v are calculated from B & G by using the relationships: Y = 9BG/ (3B +

G), v = (3B-Y)/6B,37,38

where B and G are obtained from the Voigt-Reuss-Hill (VRH) average scheme.39,40

The elastic constants of SnO under pressure (up to 25 GPa) are summarized in Table 2. The elasticity in

length is represented by elastic constant C11 (C33) which is the consequence of longitudinal strain, whereas the

shearing elasticity is related to the elastic constants C12 (C13) and C44 (C66). Figure 3(a) shows the pressure

dependence of C11, C33, C66, C12, C13 and C44. The variation of elastic constants C44, C66 show lesser sensitivity to

pressure compared to other elastic constants.

Fig. 2. The pressure dependence of the normalized lattice parameters, (a) a/a0, c/c0 and V/V0 (b) c/a of SnO.

Pressure, P (GPa)

0 5 10 15 20 25

No

rmal

ized

par

amet

ers

0.70

0.75

0.80

0.85

0.90

0.95

1.00

a/a0

c/c0

V/V0

(a)

Pressure, P (GPa)

0 5 10 15 20 25

c/a

1.10

1.15

1.20

1.25(b)

Fig. 3. (a) The pressure dependence of elastic constants Cij (GPa) and (b) anisotropic factor of litharge SnO as function of pressure.

Now let us consider the other elastic constants presented in Table 2. The bulk modulus describes the

material’s response to uniform pressure i.e., the resistance to change in volume. We see that it is more difficult

to change the volume of SnO at higher pressure because the values (B) are found to be increased with pressure.

The shear modulus G represents the resistance to elastic shear deformation and is also found to be increased at

high pressure phases. The stiffness of materials is generally expressed by its Young’s modulus Y. The higher

value of Y indicates higher stiffness of the material. It is also found that the phase under consideration is found

to be stiffer at higher pressure (see table 2). The values of C11, C33, C66, C12, C13, C44, B, G, and Y do not

indicate the measurement of the mechanical hardness of the materials but these are normally greater for

comparatively harder materials. It is found that the constants mentioned above are found to be increased with

the increase of pressure. Therefore, we can conclude that the SnO becomes harder with rise in pressure.

Brittle/ductile nature of solid can be predicted in terms of Poisson’s ratio and Pugh ration. The value of

Poisson’s ratio, ν is typically 0.33 for ductile metal and for brittle material its value is small

41. It is found that the

SnO shows ductile metallic behavior at high pressure but lies in borderline of brittle to ductile at low pressure.

Pugh42

(Pugh ratio, G/B) gave a critical value for ductile-brittle transition. For brittle materials G/B ratio is

greater than 0.5 while for ductile materials its value is less than 0.5. From Table 2, we see that SnO becomes

more ductile with increasing pressure while at low pressure (even zero pressure) it lies in borderline of brittle to

ductile transition.

Table 3. Different anisotropic constants of SnO as a function of pressure.

Pressure, P

(GPa) A

Bv (GPa)

BR (GPa)

GV (GPa)

GR (GPa)

AB AG A1 A2

0 4.666667 53 34 28 12 0.218 0.4 16 1.06

5 3.037037 78 64 44 30 0.098 0.189 6.4 1.27

10 4.071429 101 92 54 35 0.046 0.213 6.8 1.49

15 4.709677 133 124 62 40 0.035 0.215 6.7 1.93

20 5.16129 150 141 67 41 0.030 0.240 7.2 2.03

25 4.465116 166 155 76 51 0.034 0.196 5.5 2.24

Anisotropic factor of any crystal is very significant in applied science and also in crystal physics. Therefore,

it is very important to describe properly the anisotropic behavior of any materials for engineering application.

The anisotropy of atomic bonding in different planes is described by the shear anisotropic factors which are

defined by following equations for tetragonal litharge type SnO for the {1 0 0} and {0 0 1} shear planes:43

1211

661

2

CC

CA

; 133311

442

2

4

CCC

CA

.

In general for an isotropic crystal, the factors A1 and A2 must equate to one, while departure from unity

denotes the degree of elastic anisotropy. The anisotropic factors A1 and A2 as a function of pressure are plotted

in Fig. 3. It is found that A2 almost keeps constant and A1 decreases sharply up to pressure 5 GPa and becomes

Pressure, P (GPa)

0 5 10 15 20 25

Ela

stic

co

nsta

nts

(GP

a)

40

80

120

160

200

240C11

C12

C13

C33

C44

C66

(a)

0 5 10 15 20 25

Anis

otr

opic

Facto

r

0.1

0.2

0.3

0.4AB

AG

Pressure, P (GPa)

0

6

12

18

A1

A2

(b)

almost constant up to 20 GPa and thereafter decreases with pressure. The anisotropy only depends on the

symmetry of the crystal. A change in crystal structure under applied pressures has been occurred due to the

variations of lattice constants a and c at various pressures. As a result, the elastic anisotropy is also changed

because of the pressure dependence of elastic constants. The elastic anisotropy can be defined in terms of bulk

and shear modulus as, AB = (BV - BR)/(BV + BR) and AG = (GV - GR)/(GV + GR). The materials show isotropic

nature when the values of AB (BV = BR) and AG (GV = GR) become zero, while a non-zero value indicates the

anisotropy of the materials. The calculated AB and AG are also presented as a function of pressure in Fig. 3. As

the pressure increases, the anisotropy of the bulk modulus AB decreases exponentially whereas the shear

modulus anisotropy AG, decreases dramatically with pressure.

3.3. Electronic properties at 0 GPa and 5 GPa

The band structures of SnO along high-symmetry directions of the crystal Brillouin zone (BZ) are displayed in

Fig. 4 (a and b) for 0 GPa and 5 GPa only. The Fermi level is set at 0 (zero) eV in the energy scale. No

significant changes are observed in the band structures at higher pressure which are not shown in figures. The

band structure shows that the SnO is an indirect band gap semiconductor. The band gap of 0.4598 eV is found

from to M [Fig. 4(a)]. The minimum direct band gap is found to be 2.0 eV. Our results can be compared with

the values of 0.3 eV (indirect) and 2.0 eV (direct) by Errico23

using the Full-Potential Linearized Augmented-

Plane Wave (FP-LAPW) method as implement in WIEN97 code and also with the values obtained by Liu et al24

0.476 eV (indirect) and 2.0 eV (direct), by using LDA as implemented in CASTEP code. SnO is normally

known as a semimetal or a small gap semiconductor with an optical gap of 2.5-3 eV,44

where as the fundamental

gap of 0.7 eV45

is also reported. It is important to note that the pressure has enormous effect on the band gap of

SnO and the band gap very much responsive to the c/a ratio.20,23

Normally, the values of band gap energy

obtained from DFT calculation are smaller than the experimental values. We have pointed out this fact briefly in

another article18

which is based on SnO2.

The total and partial DOS for 0 & 5 GPa are shown in Fig. 5. The details study of electronic structure can be

obtained from the total and partial (DOS) of SnO. The contribution from O-p states is attributed to the band

structure around the Fermi level, EF. In order to describe the contribution from different states we sub-divide the

band below Fermi level into three energy region. The lower band around -18 eV to -20 eV is mainly derived

from O-s states while the little contribution from S-s and S-p states also noticeable. The valence band from 0 to

around -9 eV can be divided into two sub-bands and namely upper sub-band and lower sub-band. The upper

sub-band is derived mainly from O-p states down to around – 7.5 eV when a small contribution of Sn-p states is

noticeable and the lower sub-band is derived from Sn-s states. The DOS of the conduction bands are mainly

derived from Sn-p states while Sn-s and O-p states also have a little contribution.

Fig. 4. Band structure at (a) 0 GPa and (b) 5 GPa.

k-points

Energ

y,

E (

eV

)

-20

-10

0

10

20

Z A M Z R X

EF

(a)

k-points

-20

-10

0

10

20

Z A M Z R X

Energ

y,

E (

eV

)

EF

(b)

To study the pressure effects on electronic properties we now compare the band structures and density of

DOS of SnO for 0 and 5 GPa as displayed in Figure 4 and 5. Figure 4 & 5 clearly distinguish the bands and

DOS by the existence of additional features obtained at 0 & 5 GPa due to the effect of hydrostatic pressure. No

bands cross the Fermi level in the band-structure [Figure 4(a)] obtained at 0 GPa but the appearance of extra

bands in band gap region is the main feature due the pressure effects. From Fig. 4(b), it is clearly seen that the

conduction band cross significantly the Fermi level which is the evidence for the overlapping of valence band

and conduction band. Though the valence band and conduction band does not overlap directly because of the

indirect band gap of SnO. This can be explained in terms of partial density of states. In Fig. 5 (b) we can see an

additional peak of Sn-s states at the Fermi level. Also the contribution from Sn-p states at Fermi level is

increases with increasing pressure. Due to hybridization of Sn-p and Sn-s states at Fermi level at higher

pressure, SnO transform into metal from semiconductor. If we further increase the pressure no significant

change have been observed but only the value of DOS at Fermi is found to be slightly increased.

3.4. Optical properties at 0 GPa and 5 GPa

When an electromagnetic radiation is incident on the materials, different materials behave in different way. The

complex dielectric functions; 𝜀 𝜔 = 𝜀1 𝜔 + 𝑖𝜀2 𝜔 is one of the main optical characteristics of solids and the other optical constants can be obtained from it. The imaginary part ε2 (ω) is calculated in CASTEP

46

numerically by a direct evaluation of the matrix elements between the occupied and unoccupied electronic

states. The expression for the ε2 (ω) can be found elsewhere.47,48

The Kramers-Kronig relations are used to

derive the real part ε1(ω) of dielectric function. The other optical constants described in this section are derived

from ε1(ω) and ε2(ω) using the equations given in ref. 46.

The optical constants of SnO are shown in Fig. 6 (left and right panel) for (100) polarization direction. To

smears out the Fermi level for effective k-points on the Fermi surface, we used a 0.5 eV Gaussian smearing.

Similar to the electronic properties only 0 and 5 GPa data are shown because of the insignificant change in

optical properties after 5 GPa.

The electronic properties of crystalline material are mainly characterized by the imaginary part, ε2(ω) of

dielectric function, ε(ω) which depicts the probability of photon absorption. The peaks of ε2(ω) is associated

with the electron excitation. There are three peaks at 3.5, 7.8, and 15.7 eV [Fig. 6 (left panel, b)]. The main peak

at 4.5 eV may arise due to the electrons transition from O-2p and Sn-5p states. The second peak at 8 eV caused

by the electrons transition from Sn-5s states. The positions of the peaks are in good agreement with Liu et al.24

At higher pressure (5 GPa) the peaks positions is less like to be remain same. The dielectric constant ε1 (0) [Fig.

Fig. 5. Density of states (DOS) at (a) 0 GPa and (b) 5 GPa.

0

1

2

3

4Total

DO

S (

elec

trons/

eV)

0

1

2O-2s

O-2p

EF

Energy, E (eV)

-20 -10 0 10 20

0

1

2Sn-5s

Sn-5p

(a)

0

1

2

3

4Total

DO

S (

elec

tron

s/eV

)

0

1

2

O-2s

O-2p

EF

Energy, E (eV)

-20 -10 0 10 20

0

1

2 Sn-5s

Sn-5p

(b)

6 (left panel, a)] at zero energy has the value of about 7, indicating the dielectric nature of SnO. The position of

the peak (4.5 eV) is also in good agreement with Liu et al.24

At high pressure the large negative value of ε1 is a

indication of Drude-like behavior which is the characteristics of metals.

The refractive index is another technically important parameter for optical materials. The spectra for

refractive index n and the extinction coefficient k are demonstrated in Fig. 6 (left panel, c & d). The static value

of n(0) is obtained of about ~ 2.8 at 0 GPa which is comparable with that obtained by Liu et al.24

while the value

is found to be 3.3 at 5 GPa. The peaks positions and pattern of curves for refractive index and extinction

coefficient are similar to the curve obtained by Liu et al.24

Figure 6 (right panel, a & b) shows the absorption coefficient and conductivity spectra of the compound

under consideration at 0 and 5 GPa. The curves for 0 GPa delayed to start due the existence of band gap but

started in well advance for 5 GPa compared to 0 GPa showing the reduction of band gap. The results are

matched well with bands structure results. There is no significant change in the positions and height of the peaks

due to applied pressure after 5 GPa. The curve is associated with several peaks within the energy range studied.

The loss function L(), shown in Fig. 6 (right panel, c), is defined as energy loss of a electron with high

velocity passing through the materials. This curve is characterized by a peak which is known as bulk plasma

frequency P, which occurs at 2< 1 and 1 = 0. In Fig. 6 (right panel, c), The value of the effective plasma

frequency P is found to be ~ 19.3 and 20 eV for 0 and 5 GPa, respectively. The material becomes transparent,

when the frequency of incident photon is greater than P. The reflectivity curve is shown in Fig. 6 (right panel,

d). It is found that the reflectivity of the compound starts with a value of ~ 0.23 & 0.28 for 0 and 5 GPa,

respectively. After an increase with photon energy up to ~ 5 eV, the reflectivity falls again. The value of

reflectivity finally rises to reach a maximum value of ~ 0.35 and 0.48 at ~ 18 and 20 eV for 0 and 5 GPa,

respectively. The high value of reflectivity at 5 GPa compared to the value obtained at 0 GPa in very low energy

range is a sign of the increase in conductivity at higher pressure. Moreover, the peak of loss function is

associated with the trailing edges of the reflection spectra.

4. Conclusion

We have studied the structural, elastic, electronic and optical properties of SnO under high pressure. The lattice

constant c is found to be more responsive to pressure than a. The change in the c/a ratio might be attributed to

Fig. 6. Left panel: (a) ε1, (b) ε2, (c) n & k at 0 GPa, (d) n & k at 5 GPa; Right panel: (a) absorption coefficient,

(b) photoconductivity, (c) loss function, (d) reflectivity of SnO.

-40

-20

0

20

1 at 0 GPa

1 at 5 GPa

Die

lect

ric

func

tion

0

10

20

2 at 0 GPa

2 at 5 GPa

(a)

(b)

Ref

ract

ive

inde

x

0

1

2

3n at 0 GPa

k at 0 GPa

Energy, E (eV)

0 10 20 30

0

1

2

3

n at 5 GPa

K at 5 GPa

(c)

(d)

Energy, E (eV)

0 10 20 30

Ref

lect

ivit

y

0.0

0.2

0.4

3

2

1

0

Los

s fu

ncti

on

0

3

6

Abs

orpt

ion

(cm

-1)

x10

5

(c)

(a)

Con

duct

ivit

y

0

2

4(b)

(d)

the semiconductor to metal transition. The SnO is found to be mechanically stable. The elastic constant are

found to be increased with increasing pressure results an improvement of mechanical hardness. Also the SnO

becomes more ductile at higher pressure. The band structures at 0 (zero) GPa shows the semiconducting

behavior but at a higher pressure a transition to metal is found. Finally, optical properties have also been

calculated and discussed. The optical properties also distinct the transition from semiconductor to metal at zero

pressure and high pressure, respectively.

References

[1] P. F. McMillan, Nat. Mater. 1, 19 (2002). [2] R. J. Hemley and N. W. Ashcroft, Phys. Today 51, 26 (1998). [3] D. G. Isaak, Ultrahigh-Pressure Mineralogy: Physics and Chemistry of the Earth’s Deep Interior; Mineralogical Society of

America: Washington DC, 1998.

[4] R. J. Hemley, Annu. Rev. Phys. Chem. 51, 763 (2000).

[5] R. W. G. Wyckoff, Crystal Structures, Wiley, New York, 1, 1965.

[6] A. Goetzberger and C. Hebling, Sol. Energy Mater. Sol. Cells 62, 1 (2000).

[7] G. Frank, E. Kaur and H. Kostlin, Sol. Energy Mater. 8, 387 (1983).

[8] S. Cohen, Thin Solid Films 77, 127 (1981).

[9] W. Y. Chung et al., Sensors Actuators B 20 (1994) p.139.

[10] J. R. Brown et al., Sensors Actuators B 63, 109 (2000).

[11] P. Nelli et al., Thin Solid Films 371, 249 (2000).

[12] I. Stambolova et al., Mater. Chem. Phys. 63, 177 (2000).

[13] S. M. Qin et al., J. Infrared Millim. Waves 27, 101 (2008). [14] D. Calestani et al., Mater. Sci. Eng. C 25, 625 (2005). [15] Z. Lei et al., Acta Energ. Solaris Sinica 25, 624 (2004). [16] H. Zhang et al., Mater. Res. Bull. 43, 3164 (2008). [17] P. E. Lippen et al., Hyperfine Interact. 126, 137 (2000). [18] M. A. Ali and A. K. M. A. Islam, Physica B 407, 1020 (2012). [19] M. A. Bezzerrouk et al., Superlattices and Microstructures 84, 80 (2015). [20] N. E. Christensen et al., Phys. Rev. B 72, 014109 (2005). [21] H. Giefers, F. Porsch and G. Wortmann, Physica B 373, 76 (2006). [22] Y.W. Li et al., J. Phys.: Condens. Matter. 19, 425230 (2007). [23] L. A. Erric, Physica B 389, 140 (2007). [24] Q. J. Liu, Z. T. Liu and L. P. Feng, Comput. Mater. Sci. 47, 1016 (2010). [25] İ. Erdem, H. H. Kart and T. Cagin, Arch. Mater. Sci. Engg. 45, 108 (2010). [26] X. Wang et al., Phys. Status Solidi b 241, 3168 (2004). [27] M. K. Forthaus et al., Phys. Rev. Lett. 105, 157001 (2010). [28] D. M. Adams et al., Phys. Rev. B 46, 11358 (1992). [29] N. R. Ssrebryaya et al., Dokl. Akad. Nauk SSSR 187, 307(1969). [30] K. Suito, N. Kawai and Y. Masuda, Mater. Res. Bul.l 10, 677 (1975). [31] M. D. Segall, P. J. D. Lindan, M. J. Probert, C. J. Pickard, P. J.Hasnip, S. J. Clark and M. C. Payne, J. Phys.: Condens.

Matter 14, 2717 (2002).

[32] M. C. Payne, M. P. Teter, D. C. Allan, T. A. Arias and J. D. Joannopoulos, ReV. Mod. Phys. 65, 1045 (1992). [33] J. P. Perdew, K. Burke and M. Ernzerhof, Phys. Rev. Lett. 77, 3865 (1996).

[34] H. J. Monkhorst and J. D. Pack, Phys. Rev. B 13, 5188 (1976). [35] B T. H. Fischer and J. Almlöf, J. Phys. Chem. 96, 9768 (1992). [36] M. Born and K. Huang, Dynamical Theory of Crystal Lattices. Oxford, Clarendon (1956). [37] A. Bouhemadou, Braz. J. Phys. 40, 52 (2010). [38] M. A. Ali, A.K.M. A. Islam and M. S. Ali, J. Sci. Res. 4, 1 (2012). [39] R. Hill, Proc. Phys. Soc. London A 65, 349 (1952). [40] M. V. Nevitt et al., Physica B 152, 231 (1988). [41] J. Haines, J. Leger, and G. Bocquillon, Ann. Rev. Mater. Res. 31, 1 (2001). [42] S. F. Pugh, Philos. Mag. 45, 823 (1954). [43] T. Ichitsubo et al., Acta Mater. 51, 4863 (2003). [44] J. Geurts, S. Rau, W. Richter and F. J. Schmitte, Thin Solid Films 121, 217 (1984). [45] K. M. Krishna et al., Electrochim. Acta 41, 1999 (1996). [46] Materials Studio CASTEP Manual & Accelrys 2010, /http://www.tcm.phy.cam.

ac.uk/castep/documentation/WebHelp/CASTEP.htmlS.

[47] M. A. Ali, N. Jahan and A. K. M .A. Islam, J. Sci. Res. 6, 407 (2014). [48] M. A. Hadi et al., J. Sci. Res. 6, 1 (2014).